Thank you for visiting nature.com. You are using a browser version with limited support for CSS. To obtain the best experience, we recommend you use a more up to date browser (or turn off compatibility mode in Internet Explorer). In the meantime, to ensure continued support, we are displaying the site without styles and JavaScript.

# Iron phthalocyanine-sensitized magnetic catalysts for BPA photodegradation

## Abstract

The catalytic behavior of iron phthalocyanine (FePc)-sensitized magnetic nanocatalysts was evaluated for their application in the oxidative treatment of Bisphenol A (BPA) under mild environmental conditions. Two types of FePc (Fe(II)Pc and Fe(III)Pc), which are highly photosensitive compounds, were immobilized on the surface of functionalized magnetite. The nanomaterials were characterized by high resolution transmission electron microscopy (HR-TEM), X-ray diffraction (XRD), Fourier transform infrared spectroscopy (FTIR) and thermogravimetric analyses (TGA). The generation of singlet oxygen by nanomaterials was also investigated. In the presence of UVA light exposure (365 nm) and 15 mM H2O2, the M@Fe(III)Pc photocatalyst gave the best results; for a catalyst concentration of 2.0 g L − 1, around 60% BPA was removed after 120 min of reaction. These experimental conditions were further tested under natural solar light exposure, for which also M@Fe(III)Pc exhibited enhanced oxidative catalytic activity, being able to remove 83% of BPA in solution. The water samples were less cytotoxic after treatment, this being confirmed by the MCF-7 cell viability assay.

## Introduction

Emerging recalcitrant organic pollutants received extensive attention over the years, since they are difficult to remove using conventional technologies. Continuous efforts are made to find improved solutions for fighting against and for diminishing environmental pollution. Endocrine disruptive chemicals (EDC) are a class of hazardous persistent pollutants exhibiting numerous harmful effects, able to induce subtle and irreversible changes in living organisms, even in concentrations of few parts per billion1,2. Bisphenol A (BPA) is an EDC that remains a major water contaminant, since its production in the 1950s. Since then, BPA become a well-established model compound for persistent micropollutants. Although found in low concentration in water, its removal proved to be unsuccessful using conventional water treatment approaches, such as chlorination and ozonation, processes that also exhibit several draw-backs3. Promising alternatives, such as photocatalysis1,4,5,6, were found to be very efficient and versatile. For instance, photocatalysis involving dye-sensitization represents an eco-friendly approach with great potential for very efficient removal of persistent hazardous pollutants from waters. Singlet oxygen, a reactive oxygen species (ROS), has proved to be an extremely effective agent in the oxidation of emerging pollutants, due to its high oxidation ability.

Organic phthalocyanines (Pcs) are the synthetic analogues of natural porphyrine compounds7. Discovered in 1928, Pcs, possessing a two-dimensional geometry and a ring system consisting of 18 π-electrons, are composed of four isindole units linked by nitrogen atoms. Due to the large, aromatic, macrocyclic structure of Pc, a variety of metals (Me), such as Fe8,9,10, Zn11,12, Cu13,14, Mn, Co, Ni15,16, Si17, Ru18, can be bonded inside the cycle of Pc, substituting the two hydrogen atoms. These metals can tune the fine structure of the new functionalized compound as well as its physical and chemical properties. Pcs and their metalo-derivates exhibit numerous remarkable features such as excellent chemical and thermal stability, high response to light exposure in a large range from UV to near infrared region of the light spectrum, etc. Moreover, their ability to generate singlet oxygen, makes them ideal photosensitizers. Thus, they found applicability in various fields. Recent advances in phthalocyanine-based functional materials are presented in a very comprehensive review by Bian and Jiang19. A detailed review of Pc synthesis and application as catalysts is given by Sorokin20. Among application as catalysts, Pcs have been received special attention as their efficiency can potentially be increased by the presence of Fe, which may play an important role due to the redox dynamic structure of the Fe(II)/Fe(III) in oxygen reduction reaction (ORR) and photocatalysis. In literature, a limited number of studies were found about the potential of single–atom catalysts of the iron phthalocyanine (FePc) mechanism for the hydrogen peroxide activated catalytic decomposition of recalcitrant organic pollutants.

In comparison with homogeneous photocatalysis, heterogeneous photocatalysis presents significant advantages; in the latter mentioned procedures, the FePcs can be fixed onto solid supports, such as magnetic substrates, which allow easy retrieval of the material from the environment without causing additional pollution; this also provides the possibility of material reuse in subsequent water treatment cycles. Magnetite (Fe3O4) is a popular choice among magnetic carriers, being recognized as an eco-friendly material with numerous important advantages and extensive applications. The incorporation of Fe3O4 particles in polymers provides material stability, protection against oxidation, nanoparticle dispersion and possibility for further functionalization. Based on the versatile reactivity of phthalocyanine with metal and outstanding physical properties of MePc, introducing the phthalocyanine to Fe3O4 nanoparticles may result into a new hybrid material whose properties can be different not only from the single polymer but also from the Fe3O4, due to the synergistic effects derived from the interaction between them. The few reported data in the literature demonstrates that such interaction generally leads to improved photophysical and photochemical properties of MePc- Fe3O4 systems8,10,21.

Hence, in this study, we report the synthesis and photocatalytic behavior of FePc-sensitized magnetic nanoparticles for the photodegradation of BPA in solution. The combination of advanced oxidation processes with light-responsive FePc immobilized on magnetic nanoparticles was investigated for efficient BPA photodegradation at near-neutral pH, using different catalyst dosages and H2O2 concentrations, under different light sources. The obtained magnetic nanocatalysts were easy recoverable and recyclable, possessing good photocatalytic activity, especially under visible light photoactivation.

## Results and discussion

### Photocatalyst characterization

The high-resolution transmission electron microscopy analyses were used in order to reveal the morphological properties of the catalysts. HR-TEM images (Fig. 1a,b, left column) confirmed the detailed morphology and nanoscale dimension of the magnetic photocatalysts; the quasi-spherical shape of the nanoparticles, with diameters up to 15 nm, were identified in each sample, which is the typical result following the application of co-precipitation method for magnetic nanoparticle synthesis. A thin coating of ca. 1 nm was identified to surround the magnetic cores. The Selected Aria Electron Difraction (SAED) images (Fig. 1c,d, right column) confirmed that the diffraction rings belong to the magnetite crystalline phase, while the coating of the magnetite cores with organic shell is evidenced by the hollow rings.

The structure phase and average core size of the synthesized catalysts were analyzed based on the recorded XRD patterns of the obtained samples. Figure 2 shows the XRD patterns of M@Fe(II)Pc and M@Fe(III)Pc catalysts. Magnetite (Fe3O4) was the dominant crystalline phase in all samples exhibiting the typical spinel cubic structure of iron oxide. The peak positions at 2θ = 30.245°, 35.603°, 43.242°, 53.663°, 57.113°, and 62.728°, assigned to six indexed planes (2 2 0), (3 1 1), (4 0 0), (4 2 2), (5 1 1) and (4 4 0), respectively, confirm that the obtained nanoparticles consist of crystalline Fe3O4.

The narrow diffraction peaks of the obtained XRD patterns indicate that all samples consist of nanocrystals with larger average crystallite sizes of ca. 12 nm and 16 nm, for M@Fe(II)Pc, and M@Fe(III)Pc respectively; they were estimated by Scherrer’s equation from the recorded XRD data on each sample (according to the linewidth of the (3 1 1) plane refraction peak):

$${d}_{XRD}=\frac{K\lambda }{\beta \,\cos \,\theta },$$

where λ = 0.154 nm is the incident X-ray wavelength, K = 0.94 is the particle shape factor for magnetite, β is given by the full width at half-maximum of the (3 1 1) diffraction reflection and θ is the corresponding diffraction angle (here, 2θ = 35.6°). The results indicated that the capped organic layers did not change crystalline phase of Fe3O4. The XRD data is in agreement with the HR-TEM results.

Figure 3 shows the FTIR spectra of hybrid magnetic nanoparticles which were analyzed comparatively to the ones of the individual component materials. Literature findings showed that FTIR spectra of magnetite, which exhibits two strong infrared absorption bands at 570 cm−1 (υ1) and 390 cm−1(υ2), can be assigned to the Fe–O stretching mode of the tetrahedral and octahedral sites for the υ1 band and the Fe–O stretching mode of the octahedral sites for the υ2 band22. These main Fe-O vibration bands may differ as function of various factors related to magnetite synthesis protocol, oxidation, stoichiometry of magnetite (Fe(II)/Fe(III) ratios), etc23,24,25,26,27,28,29,30,31. As an example, FTIR investigation of hydrothermally synthetized magnetite showed the two absorption bands at 584 cm−1 and 442.03 cm−1 respectively32. Accounting for the above, the vibration peaks at 580 cm−1, observed in both catalysts, are assigned to Fe-O stretching vibration of Fe–O bonds of Fe at tetrahedral and octahedral sites.

The band between 1000 and 1650 cm−1 is assigned to the phthalocyanine cycle, and is related to the formation of FePc from the coordination between iron atoms and nitrogen atoms in phthalocyanine ring. The peak at 1161.9 cm−1, corresponding to variable C–N stretching33 from Fe(II)Pc, but shifted towards lower wavenumbers in the M@ Fe(II)Pc (1160.94 cm−1), as well as the peak at 1322.93 cm−1 corresponding to N–O symmetric or C–N stretching33 in Fe(II)PC, but shifted towards higher wavenumber in the M@ Fe(II)Pc (1330.64 cm−1) indicate FePc binding on to magnetite. The peak at 1498.42 cm−1 in Fe(II)Pc, corresponding to medium C-C stretching vibrations / strong C=O stretching/C–H stretching, is shown as slightly sifted at 1512.88 cm−1 in M@Fe(II)Pc (Table 1). This indicate that one of the above functional groups may contribute to Fe(II)Pc binding onto magnetite surface. The particular peak at 1418.39 cm−1 possibly being assigned to C–C stretching or C–H stretching or free O–H bending33, it is present in both, Fe(II)Pc and M@Fe(II)Pc spectra, and it seems not be involved in magnetite functioning, as it is not shifted. Specific to Fe(III)Pc are the following vibrations: 1028.84 cm−1 and 1390.42 cm−1, which are also present in the M@Fe(III)Pc, but slightly shifted toward positive wavenumbers at 1030.77 cm−1 and 1398.14 cm−1, respectively (Table 1). They indicate S=O stretching33 which contribute to Fe(III)Pc binding onto magnetite via sulfoxide groups and sulfate groups, respectively, corresponding to the molecular structure of our initial Fe(III)Pc compound. The particular peak at 1197.58 cm−1, present in both Fe(III)Pc and M@Fe(III)Pc spectra, and being assigned to S=O stretching33, may belong to another sulfate site, which seems not be involved in magnetite functioning. Vibrations observed in the interval of 1595.81 cm−1 and 1630.62 cm−1 are present in the both FePc compounds and functionalized magnetite spectra. They can be assigned to C=C stretching vibrations of atoms which are present in aromatic rings of FePc compounds. Moreover, the magnetite-PEG interaction is not evidenced by intense well-defined vibration peaks since the polymeric shell linking the FePc on the magnetic cores is very thin; however, vibration band at 1630 cm−1 as well as bands around 1400 and 1600 cm−1 might be assigned to the −CH2 and −CH3 groups and symmetric and asymmetric stretching vibration of carboxyl group, respectively, of the PEG chains34. The broad band around 3400 cm−1 corresponds to the stretching vibrations of the hydroxyl groups in the materials composition. These results indicate the formation of Fe3O4/FePc hybrid material.

The fabricated magnetic catalysts possess high saturation magnetization values as shown in our previous reports studying magnetite-based photocatalysts35. The good magnetic properties reveal that the prepared catalysts could be easily separated from reaction medium by the use of external conventional magnet without loss of the magnetic material.

The obtained TG curves of the hybrid magnetic photocatalysts are shown in Fig. 4. The results showed the weight loss steps up to 800 °C. The weight loss step over 350 °C was associated with degrading phthalocyanine.

Thus, the total weight loss was about 3.28% for the sample M, 7.01% for the M@Fe(II)Pc catalyst and 3.84% in the case of the M@Fe(III)Pc catalyst. For all the catalysts, the weight loss is including the residual water loss. At temperature above 200 °C the TG curves of the M and M@Fe(III)Pc shows a weight increase of about 0.65%, most probably due to the oxidation of the magnetite into maghemite as previously mentioned36. As shown in Fig. 4, the most pronounced mass loss, was occurred for the M@Fe(II)Pc and M@Fe(III)Pc catalysts between 200 °C and 400 °C and it is assigned to the polymer decomposition and burning. The TG curve of the M@Fe(II)Pc present a weight decrease in the temperature range from 100 °C to 400 °C and a mass increase after 400 °C. This behavior, different from the others two samples, can be due to the fact that this sample is covered by a bigger amount of polymer (7.01%), which makes it stable to oxidation over this temperature range. Thus, after the polymer is decomposed, a slight increase (0.5%) in mass occurs, which corresponds to the oxidation of the magnetite to maghemite. The weight loss difference between the M and the M@Fe(II)Pc is about 3.73%, indicating the presence of the Pc(II) polymers in the photocatalyst. In the case of the M@Fe(III)Pc photocatalyst, the difference is only of 0.56%, indicating less polymer covering the magnetite in this sample.

### Kinetics of BPA photodegradation and cytotoxicity of the samples

The effect of catalysts concentration, hydrogen peroxide concentration and the initial concentration of micropollutant, as well as the reutilization of the catalyst have been considered for the photodegradation of BPA in the present study. Additionally, the concentration of singlet oxygen has been determined.

Three concentrations of catalyst (1.0, 2.0, 3.0 g L−1) were used in our experiments. According to the results presented in Fig. 5a,b, the highest degradation has been achieved at catalyst concentration of 2 g L−1 for both catalysts, slightly more active being the M@Fe(II)Pc catalyst. The photodegradation of BPA in the presence of both catalysts is between 19 and 28%, depending on the concentration of catalysts used in the experiments.

At higher concentration of the catalyst (>2 g L−1) no improvement in the degradation of the pollutant could be observed. This could be explained by the agglomeration of magnetic nanoparticles, at higher concentration. Thus, the concentration of 2 g L−1 has been selected for the next experiments.

Under natural solar light the degradation of BPA was between 15 and 20% that is similar to degradation under UVA light (Fig. 6). In the presence of H2O2 the degradation was enhanced. 83% of BPA in solution was removed by the Fe(III)Pc photocatalyst during 120 minutes of irradiation.

Additionally, the property as a photosensitizer of the catalysts to generate singlet oxygen was investigated. The results are presented in Fig. 7. and show that, after 60 minutes of irradiation, in the presence of M@Fe(II)Pc catalyst, 9.8 µmol L−1 of singlet oxygen was generated, whereas in the presence of M@Fe(III)Pc catalyst only 1.26 µmol L−1 were produced. This indicate that the M@Fe(II)Pc catalyst can promote more efficiently the formation of 1O2, which enhances the degradation of BPA.

The proposed mechanism could be as follows: the BPA oxidation and degradation is triggered by the Reactive Oxygen Species (ROSs) generated by a molecular oxygen activation process which occurred in the presence of photosensitizer under the UV irradiation5,35,37,38,39,40,41. Detailing, a photon is adsorbed by an electronically excited singlet state which can further undergo intersystem crossing and generate longer lived excited triplet state, promoting a sensitizer. More singlet oxygen is then being produced by energy transfer towards dissolved molecular oxygen. The magnetic core generates electrons and holes in the valence band which contribute to Fenton photocatalysis.

$${{\rm{F}}{\rm{e}}}^{3+}+{{\rm{H}}}_{2}{{\rm{O}}}_{2}\to {{\rm{F}}{\rm{e}}}^{2+}+{{\rm{H}}}^{+}+{{\rm{H}}{\rm{O}}}_{2}\bullet$$
$${{\rm{Fe}}}^{3+}+{{\rm{HO}}}_{2\bullet }\to {{\rm{Fe}}}^{2+}+{{\rm{H}}}^{+}+{{\rm{O}}}_{2}$$
$${{\rm{H}}{\rm{O}}}_{2\bullet }+{{\rm{H}}}_{2}{{\rm{O}}}_{2}\to {{\rm{H}}}_{2}{\rm{O}}+{{\rm{O}}}_{2}+{\rm{O}}{\rm{H}}\bullet$$

– in reaction with FePC and UV irradiation44:

$${{\rm{Fe}}}^{3+}+{{\rm{H}}}_{2}{{\rm{O}}}_{2}+{\rm{hv}}\to {{\rm{Fe}}}^{2+}+{\rm{OH}}\bullet +{{\rm{H}}}^{+}$$

The metal phthalocyanine is photosensitized also under UV irradiation44:

$${\rm{FePC}}+{\rm{hv}}\to {{\rm{FePC}}}^{\ast }\to {{\rm{FePC}}}^{+}+{e}^{-}$$
$${{\rm{e}}}^{-}+{{\rm{H}}}_{2}{{\rm{O}}}_{2}\to {\rm{O}}{\rm{H}}\bullet +{{\rm{O}}{\rm{H}}}^{-}$$

As shown by Wu et al. and Dai et al.49,50, the conversion of Fe(III) to Fe(II) have been probably promoted by FePc. The coordination number of Fe site in FePc structure it is changed by its binding with the hydroxyl radical (as axial ligand). This leads to geometric and electronic structural variations within the FePc27, which enhance fast electron transfer for the Fe(II)/Fe(III) cycle, generates unsaturated sites for oxidants and favour potential coordination with new Fe centers51.

The reutilisation of the catalysts is very important for their application. The M/PEG @Fe(III)-Pc catalyst has been chosen for reutilisation experiments (Fig. 8).

The activity of the catalyst remains good over four runs. Moreover, no Fe leaching was detected during the degradation experiments. In the paper of Han et al.51, the removal rate of RR195 in FePc-PAN/PMS system remained similar in five successive runs, indicating the good reusability of FePc-PAN for PMS activation under visible light irradiation. In another study43, the authors found that due to the inhibition of the light absorption by intermediate accumulation on the surface of CuFePc-PAN, a 12% decline of RhB removal was observed after five running cycles. In the study of Ouedraogo et al.52 the percentage of Orange II removal only slightly decreases from 95.8 to 91.2% after the fifth cycle. Our results are in good agreement with those reported in the literature so far.

The potential toxicity of the degradation products in the reaction medium is important issue for each wastewater treatment. To exhibit cytotoxic effects after the proposed treatment, the MCF-7 cell viability assay was carryed out (Fig. 9).

The cell viability results showed that the cytotoxicity of metabolically active cells slightly increased over the studied incubation time, indicating that after treatment the samples are less cytotoxic. Compared to control, the low absorbance could be associated with the intermediates that have been detected to exhibit cytotoxic effect.

## Conclusion

In this study two types of iron phthalocyanine (FePc)-sensitized magnetic nanocatalysts were investigated for the photodegradation of BPA, an endocrine disruptive chemical (EDC), that is able to induce damages in living organisms. The quasi-spherical shape of the nanoparticles, with diameters up to 15 nm, were identified by HR-TEM. The ultrathin coating of phthalocyanine ring of ca 1 nm surrounding the magnetic cores was also evidenced and confirmed by FTIR spectra and TG analysis. XRD patterns of the obtained samples confirmed that magnetite was the dominant crystalline phase in all samples. In the presence of M@Fe(II)Pc catalyst, 9.8 µmol L−1 of singlet oxygen was generated after 60 minutes of irradiation, whereas in the presence of M@Fe(III)Pc catalyst only 1.26 µmol L−1 were produced. The optimum concentrations of catalyst and hydrogen peroxide were 2.0 g L−1 and 15 mmol L−1 H2O2, respectively. The photodegradation of BPA in the presence of both catalysts was between 19 and 28%, whereas, with the addition of H2O2, the BPA removal have increased (between 49 and 83%) and it was accelerated by exposure to natural solar light. In the presence of hydrogen peroxide, the M@Fe(III)Pc catalyst was more active. The activity of both catalysts remains good over four consecutive runs. The MCF-7 cell viability assay showed that, after treatment, the water samples were less cytotoxic. Our results showed that both catalysts can be successfully applied in wastewater treatment.

## Methods

### Materials and characterization methods

All aqueous solutions were prepared with fresh ultrapure water (0.055 µS cm−1) produced by an Evoqua LABOSTAR Pro TWF UV unit. High purity chemicals (SIGMA-ALDRICH) were used in all experimental procedures. Iron(II) phthalocyanine (Fe(II)Pc) and iron(III) phthalocyanine-4,4′,4′′,4′′′-tetrasulfonic acid with oxygen monosodium salt hydrate (Fe(III)Pc) were chosen as sensitizers and were immobilized on magnetic nanoparticles in order to catalyse the photooxidation of BPA in solution.

A BANDELINE SONOPULS homogenizing system, model HD4100, equipped with a HF generator GM 4100, ultrasonic converter UW100, standard horn SH 100 G and a 13 mm titanium probe, was set-up at 20 W for the sonochemical synthesis of the magnetic nanoparticles.

The synthesis of the photocatalysts was followed by the characterization of their physico-chemical properties. Ultra-high resolution transmission electron microscopy (UHR-TEM) images were acquired by a LIBRA200MC/CARL ZEISS GmbH instrument (Germany). X-ray diffraction (XRD) patterns were recorded by a BRUKER AXS D8-Advance X-ray diffractometer (Germany) using Bragg-Brentano configuration and the Cu-Kα radiation (λ = 0.154 nm); the DIFFRACplus Eva software was also used in order to estimate the average crystallite size in the synthesized nanomaterials based on Scherrer’s equation. Standard Si material and its spectra was used as a reference material for FWHM analyses and calculation of relative particle size. The immobilization of phthalocyanines on the magnetic cores was evaluated by Fourier transform infrared (FT-IR) spectroscopy (JASCO 6100 spectrometer) at room temperature; powder samples prepared in KBr discs were used to record the FT-IR spectra between 400 and 4000 cm−1, with a resolution of 4 cm−1. Thermogravimetric analyses (TGA) were carried out in argon atmosphere using a NETZSCH STA 409 PC/PG device, in the temperature range from 20 °C to 800 °C with a heating rate of 5 K min−1. Electron spin resonance (ESR) spectra were recorded using a MINISCOPE MS300 device (Magnettech GmbH, Berlin, Germany) and the diamagnetic 2,2,6,6-tetramethyl-4-piperidinol (TMP-OH, 40 mmol L−1) as trap for the molecular singlet oxygen (1O2) generated in solution in the presence of the photocatalysts; the entire settings and method is described in detail in our previous work35.

### Photocatalyst synthesis

The preparation of the two photocatalysts consisted in a multi-step procedure, starting with the sonochemical synthesis of the magnetite (Fe3O4) cores and their subsequent stabilization with low molecular polyethylene glycol (PEG), immediately followed by the sensitizing of the obtained nanoparticles with photoactive compounds, namely iron phthalocyanines (FePc). The detailed procedure was described in our recent study35. Briefly, in here, the conventional wet co-precipitation route, a very efficient method for Fe3O4 nanoparticles synthesis, was carried out under ultrasound irradiation, maintaining a constant temperature of 60 °C, and normal atmospheric conditions. The as-synthesized bare magnetic nanoparticles were then rapidly functionalized with PEG in order to prevent their agglomeration and oxidation, yielding Fe3O4/PEG nanoparticles, further denoted as M. Equal amounts from the fresh black slurry M were further functionalized with either Fe(II)Pc or Fe(III)Pc. A volume of 20 mL of 3.72 mmol L−1 solution of each iron phthalocyanine was gradually poured onto 0.5 g of M and kept under rapid continuous mechanical stirring and heating (70 °C) for 210 minutes. The resulted magnetic photocatalysts, M@Fe(II)Pc and M@Fe(III)Pc respectively, were finally purified (by repeated rinsing with ultrapure water and absolute ethanol alternated with magnetic decantation for removing the residual products) then dried in an oven under vacuum at 60 °C.

### Catalytic activity

Kinetic experiments were carried out at laboratory-scale, in mild conditions (i.e. initial near-neutral pH of 6.6, room temperature 23 ± 2 °C) in order to assess the catalytic activity of the FePc-based photocatalysts for the BPA degradation in aqueous solution. A solution of 2 µmol L−1 BPA was used as initial concentration. Before starting the kinetic experiments, the catalysts was tested in the dark in the presence of BPA; the solution was analyzed at regular time intervals indicating that no adsorption phenomena occurred. Next, the photooxidation tests were carried out in 50-mL Berzelius glasses, each one containing 5 mL pollutant solution, placed on a cooled support and under a UVA light source (Analytik Jena bench lamp, λ = 365 nm, 15 W) consisting in two parallel self-filtering, low pressure ‘black light’ tubes; the diameter of the irradiated surface area was 11.34 cm2, the irradiation path-length was 0.8 cm, and photon flow of 9.28 × 10−8 Einstein s−1 (measured by polychromatic actinometry with phenylglyoxylic acid in AcN:H2O = 3:1 v/v)53. In the case of natural solar light exposure experiments, the same protocol was followed the diameter of the irradiated surface area was the same and photon flow was 9.67 × 10−8 Einstein s−1. The experiments were performed in July 2019, Iasi (47° 9′ 6.2136″ N, 27° 35′ 16.4904″ E), Romania.

The catalytic performance of the synthesized photocatalysts was assessed by evaluating the effect of catalyst concentration, hydrogen peroxide dosage, under light exposure for a total reaction time of 120 min. Catalyst concentration of 1.0, 2.0 and 3.0 g L−1 were tested in the BPA degradation experiments at various time intervals with in the total reaction time of 120 min. Five H2O2 concentrations, 5, 10, 15, 20 and 25 mmol L−1, freshly prepared from a 30% H2O2 standard solution, were studied in the next step. During kinetic experiments, aliquots of 300 μl of BPA solution were withdrawn from the reaction vessels at different time intervals (15, 30, 60 and 120 min), immediately filtered through a 0.22 µm Millipore nitro-cellulose membrane. The concentration of BPA in the supernatant solutions was determined by a high performance liquid chromatograph (HPLC-UV-VIS/DAD Agilent Technologies 1260 Infinity series). The description of experimental set-up and detailed method of analyses can be found in our previous study54. The experiments were performed in duplicate, the calculated relative standard error being under 3%.

For determination of the dissolved iron, the Ferrozine method was used55.

The detailed procedure of the MCF-7 cell viability assay, performed on the studied samples in order to test their cytotoxicity level, is described in our earlier publications37,56.

## Data availability

All data generated or analysed during this study are included in this published article.

## References

1. Zhou, D., Wu, F., Deng, N. & Xiang, W. Photooxidation of bisphenol A (BPA) in water in the presence of ferric and carboxylate salts. Water Research 38, 4107–4116, https://doi.org/10.1016/j.watres.2004.07.021 (2004).

2. Rubin, B. S., Sonnenschein, C., Vandenberg, L. N., Maffini, M. V. & Soto, A. M. Bisphenol-A and the Great Divide: A Review of Controversies in the Field of Endocrine Disruption. Endocrine Reviews 30, 75–95, https://doi.org/10.1210/er.2008-0021 (2009).

3. Reddy, P. et al. Photocatalytic degradation of bisphenol A in aqueous media: A review. Journal of Environmental Management 213, 189–205, https://doi.org/10.1016/j.jenvman.2018.02.059 (2018).

4. Sharma, J., Mishra, I. M. & Kumar, V. Mechanistic study of photo-oxidation of Bisphenol-A (BPA) with hydrogen peroxide (H2O2) and sodium persulfate (SPS). Journal of Environmental Management 166, 12–22, https://doi.org/10.1016/j.jenvman.2015.09.043 (2016).

5. Nadejde, C. et al. Hybrid iron-based core-shell magnetic catalysts for fast degradation of bisphenol A in aqueous systems. Chemical Engineering Journal 302, 587–594, https://doi.org/10.1016/j.cej.2016.05.090 (2016).

6. Xu, J., Zhao, C., Wang, T., Shaojie, Y. & Liu, Z. Photo-Oxidation of Bisphenol A in Aqueous Solutions at Near Neutral pH by a Fe(III)-Carboxylate Complex with Oxalacetic Acid as a Benign Molecule. Vol. 23 (2018).

7. Jiang, J. Functional Phthalocyanine Molecular Materials. Vol. 135 Jiang, Jianzhuang (Springer, Berlin, Heidelberg), (2010).

8. Meng, F. et al. One-step synthesis of Fe-phthalocyanine/Fe3O4 hybrid microspheres. Materials Letters 65, 264–267, https://doi.org/10.1016/j.matlet.2010.09.075 (2011).

9. Kluson, P. et al. Environmentally friendly phthalocyanine catalysts for water decontamination-Non-photocatalytic systems. Applied Catalysis B-Environmental 91, 605–609, https://doi.org/10.1016/j.apcatb.2009.06.033 (2009).

10. Tao, X., Ma, W., Zhang, T. & Zhao, J. Efficient photooxidative degradation of organic compounds in the presence of iron tetrasulfophthalocyanine under visible light irradiation. Angewandte Chemie-International Edition 40, 3014-3016, 10.1002/1521-3773(20010817)40:16<3014::AID-ANIE3014>3.0.CO;2-M (2001).

11. Cui, L. Y. et al. Synthesis, crystal structure and characterization of a new zinc phthalocyanine complex. Journal of Molecular Structure 827, 149–154, https://doi.org/10.1016/j.molstruc.2006.05.030 (2007).

12. Guo, Z. C. et al. Zinc phthalocyanine hierarchical nanostructure with hollow interior space: Solvent-thermal synthesis and high visible photocatalytic property. Journal of Colloid and Interface Science 348, 37–42, https://doi.org/10.1016/j.jcis.2010.04.035 (2010).

13. Reetz, M. T. & Jiao, N. Copper–Phthalocyanine Conjugates of Serum Albumins as Enantioselective Catalysts in Diels–Alder Reactions. Angewandte Chemie International Edition 45, 2416–2419, https://doi.org/10.1002/anie.200504561 (2006).

14. Mele, G. et al. Photocatalytic degradation of 4-nitrophenol in aqueous suspension by using polycrystalline TiO2 impregnated with functionalized Cu(II)–porphyrin or Cu(II)–phthalocyanine. Journal of Catalysis 217, 334–342, https://doi.org/10.1016/S0021-9517(03)00040-X (2003).

15. Bartolome, J., Carlos, M. & Ivan, S. Magnetism of Metal Phthalocyanines. In NanoScience and Technology 221–245, https://doi.org/10.1007/978-3-642-40609-6_9 (2014).

16. Swarbrick, J. C., Weng, T.-C., Schulte, K., Khlobystov, A. N. & Glatzel, P. Electronic structure changes in cobalt phthalocyanine due to nanotube encapsulation probed using resonant inelastic X-ray scattering. Physical Chemistry Chemical Physics 12, 9693–9699, https://doi.org/10.1039/C002501A (2010).

17. Farren, C., FitzGerald, S., Bryce, M. R., Beeby, A. & Batsanov, A. S. Synthesis, structure and optical characterisation of silicon phthalocyanine bis-esters. Journal of the Chemical Society, Perkin Transactions 2, 59–66, https://doi.org/10.1039/B108778A (2002).

18. Rawling, T. & McDonagh, A. Ruthenium phthalocyanine and naphthalocyanine complexes: Synthesis, properties and applications. Coordination Chemistry Reviews 251, 1128–1157, https://doi.org/10.1016/j.ccr.2006.09.011 (2007).

19. Bian, Y. Z. & Jiang, J. Z. in 50 Years of Structure and Bonding - the Anniversary Volume Vol. 172 Structure and Bonding (ed. D. M. P., Mingos) 159–199 (Springer), (2016).

20. Sorokin, A. B. Phthalocyanine Metal Complexes in Catalysis. Chemical Reviews 113, 8152–8191, https://doi.org/10.1021/cr4000072 (2013).

21. Kluson, P. et al. Sulphonated phthalocyanines as effective oxidation photocatalysts for visible and UV light regions. Journal of Molecular Catalysis a-Chemical 272, 213–219, https://doi.org/10.1016/j.molcata.2007.03.024 (2007).

22. Ishii, M., Nakahira, M. & Yamanaka, T. Infrared absorption spectra and cation distributions in (Mn, Fe)3O4. Solid State Communications 11, 209–212, https://doi.org/10.1016/0038-1098(72)91162-3 (1972).

23. Mazrouaa, A. M., Mohamed, M. G. & Fekry, M. Physical and magnetic properties of iron oxide nanoparticles with a different molar ratio of ferrous and ferric. Egyptian Journal of Petroleum 28, 165–171, https://doi.org/10.1016/j.ejpe.2019.02.002 (2019).

24. Ngo, T. H. et al. Facile and solvent-free routes for the synthesis of size-controllable Fe3O4nanoparticles. Advances in Natural Sciences: Nanoscience and Nanotechnology 1, 035001, https://doi.org/10.1088/2043-6254/1/3/035001 (2010).

25. Nguyen, Q., Quyen, D. & Hoang, T. A new route of emulsifier-free emulsion polymerization for the preparation of polymer coated magnetite nanoparticles. Materials Science-Poland 32, 264–271, https://doi.org/10.2478/s13536-013-0172-y (2014).

26. Nidá, S. M. & Akl, A. M. A Novel Approach for Synthesis Magnetite Nanoparticles at Ambient. Temperature. Nanoscience and NanotechnologY 3, 35–39 (2013).

27. Cao, R. et al. Promotion of oxygen reduction by a bio-inspired tethered iron phthalocyanine carbon nanotube-based catalyst. Nature Communications 4, 7, https://doi.org/10.1038/ncomms3076 (2013).

28. Cao, X., Zhang, B., Zhao, F. & Feng, L. Synthesis and Properties of MPEG-Coated Superparamagnetic Magnetite Nanoparticles. Journal of Nanomaterials 2012, https://doi.org/10.1155/2012/607296 (2012).

29. Gotić, M. & Musić, S. Mössbauer, FT-IR and FE SEM investigation of iron oxides precipitated from FeSO4 solutions. Journal of Molecular Structure 834–836, 445–453, https://doi.org/10.1016/j.molstruc.2006.10.059 (2007).

30. Namduri, H. & Nasrazadani, S. Quantitative analysis of iron oxides using Fourier transform infrared spectrophotometry. Corrosion Science 50, 2493–2497, https://doi.org/10.1016/j.corsci.2008.06.034 (2008).

31. Galhoum, A. A. et al. Cysteine-Functionalized Chitosan Magnetic Nano-Based Particles for the Recovery of Light and Heavy Rare Earth Metals: Uptake Kinetics and Sorption Isotherms. Nanomaterials (Basel, Switzerland) 5, 154–179, https://doi.org/10.3390/nano5010154 (2015).

32. Damodharan, S., Rajan, R., Veerachamy, S., A, M. & Raj, A. Synthesis and Characterization of Pullulan Acetate Coated Magnetic Nanoparticle for Hyperthermic Therapy. Procedia materials science 10, 2–9, https://doi.org/10.1016/j.mspro.2015.06.017 (2015).

33. LibreTexts. Infrared_Spectroscopy_Absorption_Table, https://chem.libretexts.org/Bookshelves/Ancillary_Materials/Reference/Reference_Tables/Spectroscopic_Parameters/Infrared_Spectroscopy_Absorption_Table (2019).

34. Gao, C., Chen, S., Quan, X., Yu, H. & Zhang, Y. Enhanced Fenton-like catalysis by iron-based metal organic frameworks for degradation of organic pollutants. Journal of Catalysis 356, 125–132, https://doi.org/10.1016/j.jcat.2017.09.015 (2017).

35. Neamtu, M., Nadejde, C., Hodoroaba, V. D., Schneider, R. J. & Panne, U. Singlet oxygen generation potential of porphyrin-sensitized magnetite nanoparticles: Synthesis, characterization and photocatalytic application. Applied Catalysis B-Environmental 232, 553–561, https://doi.org/10.1016/j.apcatb.2018.03.079 (2018).

36. Franger, S. et al. Large influence of the synthesis conditions on the physico-chemical properties of nanostructured Fe3O4. Journal of Nanoparticle Research 9, 389–402, https://doi.org/10.1007/s11051-006-9105-6 (2007).

37. Neamtu, M. et al. Functionalized magnetic nanoparticles: Synthesis, characterization, catalytic application and assessment of toxicity. Scientific Reports 8, 11, https://doi.org/10.1038/s41598-018-24721-4 (2018).

38. Legrini, O., Oliveros, E. & Braun, A. M. Photochemical Processes for Water-Treatment. Chemical Reviews 93, 671–698 (1993).

39. Neamtu, M. et al. Removal of pollutants by the new Fenton-like highly active catalysts containing an imidazolium salt and a Schiff base. Applied Catalysis B-Environmental 183, 335–342, https://doi.org/10.1016/j.apcatb.2015.10.032 (2016).

40. Nadejde, C. et al. Green Fenton-like magnetic nanocatalysts: Synthesis, characterization and catalytic application. Applied Catalysis B-Environmental 176, 667–677, https://doi.org/10.1016/j.apcatb.2015.04.050 (2015).

41. Thomas, A. H. et al. Singlet oxygen ((1)Delta(g)) production by pterin derivatives in aqueous solutions. Photochemical & Photobiological Sciences 2, 245–250 (2003).

42. Han, Z. B., Han, X., Zhao, X. M., Yu, J. T. & Xu, H. Iron phthalocyanine supported on amidoximated PAN fiber as effective catalyst for controllable hydrogen peroxide activation in oxidizing organic dyes. Journal of Hazardous Materials 320, 27–35, https://doi.org/10.1016/j.jhazmat.2016.08.004 (2016).

43. Han, X., Han, Z. B., Li, J. F., Zhao, J. & Zhao, X. M. Coordinative integration of copper (II) and iron (II) phthalocyanine into amidoximated PAN fiber for enhanced photocatalytic activity under visible light irradiation. Journal of Colloid and Interface Science 533, 333–343, https://doi.org/10.1016/j.jcis.2018.08.076 (2019).

44. Wang, Q. L. et al. Iron phthalocyanine-graphene donor-acceptor hybrids for visible-light-assisted degradation of phenol in the presence of H2O2. Applied Catalysis B-Environmental 192, 182–192, https://doi.org/10.1016/j.apcatb.2016.03.047 (2016).

45. Alvaro, M., Carbonell, E., Espla, M. & Garcia, H. Iron phthalocyanine supported on silica or encapsulated inside zeolite Y as solid photocatalysts for the degradation of phenols and sulfur heterocycles. Applied Catalysis B-Environmental 57, 37–42, https://doi.org/10.1016/j.apcatb.2004.10.003 (2005).

46. Norman, M., Zoltowska-Aksamitowska, S., Zgola-Grzeskowiak, A., Ehrlich, H. & Jesionowski, T. Iron(III) phthalocyanine supported on a spongin scaffold as an advanced photocatalyst in a highly efficient removal process of halophenols and bisphenol A. Journal of Hazardous Materials 347, 78–88, https://doi.org/10.1016/j.jhazmat.2017.12.055 (2018).

47. Rodriguez, E. M. et al. Efficiency of different solar advanced oxidation processes on the oxidation of bisphenol A in water. Applied Catalysis B-Environmental 95, 228–237, https://doi.org/10.1016/j.apcatb.2009.12.027 (2010).

48. Yang, X. J. et al. Modeling and kinetics study of Bisphenol A (BPA) degradation over an FeOCl/SiO2 Fenton-like catalyst. Catalysis Today 276, 85–96, https://doi.org/10.1016/j.cattod.2016.01.002 (2016).

49. Wu, F. et al. Visible-light-assisted peroxymonosulfate activation and mechanism for the degradation of pharmaceuticals over pyridyl-functionalized graphitic carbon nitride coordinated with iron phthalocyanine. Applied Catalysis B-Environmental 218, 230–239, https://doi.org/10.1016/j.apcatb.2017.06.057 (2017).

50. Dai, D. J. et al. Highly efficient removal of organic contaminants based on peroxymonosulfate activation by iron phthalocyanine: mechanism and the bicarbonate ion enhancement effect. Catalysis Science &. Technology 7, 934–942, https://doi.org/10.1039/c6cy02317g (2017).

51. Han, Z. B., Li, J. F., Han, X., Ji, X. J. & Zhao, X. M. A comparative study of iron-based PAN fibrous catalysts for peroxymonosulfate activation in decomposing organic contaminants. Chemical Engineering Journal 358, 176–187, https://doi.org/10.1016/j.cej.2018.09.224 (2019).

52. Ouedraogo, S. et al. Copper octacarboxyphthalocyanine as sensitizer of graphitic carbon nitride for efficient dye degradation under visible light irradiation. Applied Catalysis a-General 563, 127–136, https://doi.org/10.1016/j.apcata.2018.06.036 (2018).

53. Defoin, A. et al. A New Liquid-Phase Actinometer - Quantum Yield and Photo-Cidnp Study of Phenylglyoxylic Acid in Aqueous-Solution. Journal of Photochemistry 33, 237–255 (1986).

54. Rambu, A. P., Nadejde, C., Schneider, R. J. & Neamtu, M. Thin films containing oxalate-capped iron oxide nanomaterials deposited on glass substrate for fast Fenton degradation of some micropollutants. Environmental Science and Pollution Research 25, 6802–6813, https://doi.org/10.1007/s11356-017-1022-y (2018).

55. Viollier, E., Inglett, P. W., Hunter, K., Roychoudhury, A. N. & Van Cappellen, P. The ferrozine method revisited: Fe(II)/Fe(III) determination in natural waters. Applied Geochemistry 15, 785–790, https://doi.org/10.1016/s0883-2927(99)00097-9 (2000).

56. Rata, D. M. et al. “In vitro” behaviour of aptamer-functionalized polymeric nanocapsules loaded with 5-fluorouracil for targeted therapy. Materials Science & Engineering C-Materials for Biological Applications 103, 11, https://doi.org/10.1016/j.msec.2019.109828 (2019).

57. Chirita, M., Radu, B., Adrian, I. & Ioan, G. Superparamagnetic Unusual Behavior of Micrometric Magnetite Monodisperse Monocrystals Synthesized by Fe-EDTA Thermal Decomposition. Particulate Science and Technology - Particulate Sci Technology 30, https://doi.org/10.1080/02726351.2011.585220 (2012).

58. Fischer, G., Cao, X., Cox, N. & Francis, M. The FT-IR spectra of glycine and glycylglycine zwitterions isolated in alkali halide matrices. Chemical Physics 313, 39–49, https://doi.org/10.1016/j.chemphys.2004.12.011 (2005).

59. Andy, B. Compound Interests, https://www.compoundchem.com/2015/02/05/irspectroscopy/ (2015).

60. Newman, R. Some Applications of Infrared Spectroscopy in the Examination of Painting Materials. Journal of the American Institute for Conservation 19, 42–62, https://doi.org/10.1179/019713679806028977 (1979).

## Acknowledgements

This research did not receive any specific funding. The authors thank BAM Institute for the support of the guest scientist Dr. M. Neamțu. The authors also acknowledge the contributions of and thank Eng. M. Porcescu (XRD analyses), Dr. M. Găburici (FTIR recordings), Dr. G. Ababei (TEM recordings) from National Institute of Research and Development for Technical Physics (Iași, Romania). The article-processing charge is covered by the Ministry of Research and Innovation within Program 1 – Development of the national RD system, Subprogram 1.2 – Institutional Performance – RDI excellence funding projects, Contract no. 34PFE/19.10.2018.

## Author information

Authors

### Contributions

M.N., C.N. and L.B. conceived and designed the experiments. M.N. supervised the study. C.N. carried out materials syntheses. M.N. and L.B. performed all kinetic (photo)degradation tests and related measurements and interpretation of results. O.D. conducted FTIR and TGA characterization and data interpretation. C.N. and O.D. assessed the material properties. A.P. conducted ESR analysis and data interpretation. D.G. executed cytotoxicity tests and data analysis. All authors discussed the results, co-wrote and edited the manuscript. All authors reviewed and approved the manuscript.

### Corresponding author

Correspondence to Mariana Neamtu.

## Ethics declarations

### Competing interests

The authors declare no competing interests.

Publisher’s note Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.

## Rights and permissions

Reprints and Permissions

Neamtu, M., Nadejde, C., Brinza, L. et al. Iron phthalocyanine-sensitized magnetic catalysts for BPA photodegradation. Sci Rep 10, 5376 (2020). https://doi.org/10.1038/s41598-020-61980-6

• Accepted:

• Published:

• DOI: https://doi.org/10.1038/s41598-020-61980-6

• ### Advanced removal of Reactive Yellow 84 azo dye using functionalised amorphous calcium carbonates as adsorbent

• Loredana Brinza
• Andreea Elena Maftei
• Mariana Neamtu

Scientific Reports (2022)

• ### Fe(II)-phthalocyanine supported on chitosan aerogel as a catalyst for oxidation of alcohols and alkyl arenes

• Fatemeh Azimi

Scientific Reports (2021)